Passive Damping Characteristics of Carbon Epoxy Composite Plates


 Claire Page
 1 years ago
 Views:
Transcription
1 Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty of Mechanical Engineering, JNT University Kakinada, Kakinada533 3, India Abstract: Vibration damping is an important phenomenon in the field of engineering design while predicting the dynamic analysis of the most of the structures. It is one of the typical dynamic responses of structural members, which allows the members fail due to larger amplitudes. Composite materials are replacing conventional structural materials due to attractive, superior mechanical properties such as high strength to weight ratio, high modulus, high corrosion resistance and good fatigue resistance. Composite materials possess high degree of material damping compared with conventional materials. One of the advanced technique employed to safe guard against the severe intensity of vibrations by controlling the dynamics of the structures is the provision of enhancing energy dissipation by the design of a constrain layer. When a constrain layer is made of a non actuating stiff layer of material introduced in the structure, say a viscoelastic material called a PCLD (Passive constrained layer damping). In the present work, an analytical solution for damping of a FRP (Fiber reinforced polymer) plates with a single or double interleaved viscoelastic layers in is obtained. Ritz method is employed to predict the damping nature of the plate under several boundary conditions. Specific damping capacity and a loss factor are deduced from the method of energy formulation for viscoelastic layers interleaved in laminated fiber reinforced plate. The loss factor of constrain layered plate is calculated as a function of fiber orientation in its orthotropic layers. An isotropic constrain layers are configured at midplane, symmetric, asymmetric and outer positions across the thickness of the plate. A parametric study also carried out to observe the effect of position of a constant thickness viscoelastic layer on the damping characteristics of passively constrain orthotropic plate. Key words: Thin plate theory, specific damping capacity, loss factor and viscoelastic materials. Nomenclature U: Energy dissipated : Maximum strain energy : Fourier Coefficient of deflection : Aspect ratio : Viscoelastic layer of thickness a: Length of the plate b: Width of the plate e: Thickness of the orthotropic lamina : Reduced stiffness constants : Up Distance of VEL from laminate Midplane : Down of VEL from laminate Midplane : Transverse displacement : Series Coefficient : Product of integrals I and J : Time E: Young s modulus : Bending Moment in y direction * Corresponding author: Dileep Kumar K, assistant professor, research field: damping of composite structure. : Orientation function Greek Letters : Poisons ratio of VEM : Specific Damping Coefficient λ m: Boundary values of the plate in xdirection γ m: Boundary values of the plate in ydirection : Loss factor : Longitudinal modulus : A constant for VEM position Up Distance : A constant for VEM position down Distance. Introduction Nowadays an increased demand for the control of acoustics and vibration in structures had enforced the designers to take damping into account even from the preliminary design phase. A designer always looks for a material which shows superior or optimum properties under given operating environment. It is very difficult task to search for an optimal material for
2 36 every new design. In such cases a composite material will be the best practical solution owing to reason that its properties can be tailored according to desired degree of magnitude by providing geometric and material symmetry conditions. The advantages of composites can be made utilized by the rational choice of stacking sequence. In many aerospace, commercial and automotive components, sports and structures composites have been successfully used. Advanced composite materials not only have high stiffness but also have greater damping capacity compared to metals. For example, in a FRP composite, the damping is enhanced due to the internal friction among the constituents and interfacial slip at the fibermatrix interfaces, where as the fiber contributes to the stiffness. However, the damping capacity of the composite laminates can be increased many fold by incorporating viscoelastic layers between the laminae of the host composite. In this hybrid approach, the dominant mechanism of damping is the shear induced between the damping layer and the constraining layers. The tradeoffs in using damping layers are a slight reduction in stiffness and a small increase in the weight of the composite system. The desirable damping characteristics and design flexibility make the viscoelastic materials to be embedded as an important isotropic constituent layer in the composites. Adams R D [] consider the basic elasticity relationships for unidirectional composites, together with the AdamsBacon damping criterion, are utilised for prediction of moduli and flexural damping of anisotropic CFRP (Carbon fiber reinforced polymer) and GRP beams with respect to fibre orientation. Billups E K [] works on several twodimensional theories for investigating the SDC (Specific damping capacity) of composite materials and theories are compared with those of Adams and Bacon, Adams and Maheri, Ni and Adams [3] and Saravanos and Chamis. No interlaminar effects are considered. The analysis considers the variations of Young s modulus and damping of viscoelastic layers with the frequency. Finally, the article presents the effects of Young s modulus and the damping of a viscoelastic layer interleaved in the middle plane of unidirectional laminate by JeanMarie Berthelot [4]. The optimal layup design problem, a layer wise optimization (LO) method is applied to the orthotropic plates comprised of two different laminates, and an optimal fiber angles are determined to obtain the maximum loss factor in the first mode by Jinqiang Li [5]. JeanMarie Berthelot [6] also predicted various damping parameters and are investigated using cantilever beam test specimens using an impulse hammer technique. Damping modeling is developed by a finite element analysis which evaluated the different energies dissipated in the material as a function of fiber directions of the layers is the work of Ni, R. G. and Adams, R. D [7]. Advanced FRP composites are prime candidates for several interesting applications where damping is a key parameter. Improvement of vibration damping characteristics of such materials makes them qualify even more attractive applications. Since most of composite structural elements in military, automotive and space applications are subject to severe dynamic loads an additional vibration control becomes necessary. This can be achieved by using different damping treatments. High degree of damping in a structure can often improve performance in a dynamic load environment. Various methods for predicting damping in a structure are proposed, the Ritz method is the most efficient method. In composite base structures, several factors influence its structural vibration response. For example, the constituents, the fiber orientation and stacking sequence in the host structure, and the position from midplane, amount and type of treatment of embedded layer, influence the response strongly. The effect of some of such parameters is presented here using Ritz method.
3 37. Modeling of FRP Plate Using Ritz Method shown in Fig.. Among various passive damping layer of thickness e interleaved in the middle plane of laminates (Fig. ) and laminates with two viscoelastic layers of thickness e interleaved away from the middle plane (). The layers of the initial. Interlaminar Viscoelastic Layer viscoelastic layer of thickness e is interleaved (Fig. ). Material directions make an angle θ with the plate with the viscoelastic layers can be U = U +U + U + U 66,,,66 () The energies U and U are the strain energies directions, U is the coupling energy induced by the energy stored in the orthotropic layer and the strain energy stored in the viscoelastic layer. layers and 3 (Fig. ) can be written as () of the plate, and are the strain energies stored in layers and 3, are the reduced stiffness constants of the materials, and are functions of Fig. 37. Modeling of FRP Plate Using Ritz Method shown in Fig.. Among various passive damping layer of thickness e interleaved in the middle plane of laminates (Fig. ) and laminates with two viscoelastic layers of thickness e interleaved away from the middle plane (). The layers of the initial. Interlaminar Viscoelastic Layer viscoelastic layer of thickness e is interleaved (Fig. ). Material directions make an angle θ with the plate with the viscoelastic layers can be U = U +U + U + U 66,,,66 () The energies U and U are the strain energies directions, U is the coupling energy induced by the energy stored in the orthotropic layer and the strain energy stored in the viscoelastic layer. layers and 3 (Fig. ) can be written as () of the plate, and are the strain energies stored in layers and 3, are the reduced stiffness constants of the materials, and are functions of Fig. 37. Modeling of FRP Plate Using Ritz Method shown in Fig.. Among various passive damping layer of thickness e interleaved in the middle plane of laminates (Fig. ) and laminates with two viscoelastic layers of thickness e interleaved away from the middle plane (). The layers of the initial. Interlaminar Viscoelastic Layer viscoelastic layer of thickness e is interleaved (Fig. ). Material directions make an angle θ with the plate with the viscoelastic layers can be U = U +U + U + U 66,,,66 () The energies U and U are the strain energies directions, U is the coupling energy induced by the energy stored in the orthotropic layer and the strain energy stored in the viscoelastic layer. layers and 3 (Fig. ) can be written as () of the plate, and are the strain energies stored in layers and 3, are the reduced stiffness constants of the materials, and are functions of Fig. 37. Modeling of FRP Plate Using Ritz Method shown in Fig.. Among various passive damping layer of thickness e interleaved in the middle plane of laminates (Fig. ) and laminates with two viscoelastic layers of thickness e interleaved away from the middle plane (). The layers of the initial. Interlaminar Viscoelastic Layer viscoelastic layer of thickness e is interleaved (Fig. ). Material directions make an angle θ with the plate with the viscoelastic layers can be U = U +U + U + U 66,,,66 () The energies U and U are the strain energies directions, U is the coupling energy induced by the energy stored in the orthotropic layer and the strain energy stored in the viscoelastic layer. layers and 3 (Fig. ) can be written as () of the plate, and are the strain energies stored in layers and 3, are the reduced stiffness constants of the materials, and are functions of Fig. 37. Modeling of FRP Plate Using Ritz Method shown in Fig.. Among various passive damping layer of thickness e interleaved in the middle plane of laminates (Fig. ) and laminates with two viscoelastic layers of thickness e interleaved away from the middle plane (). The layers of the initial. Interlaminar Viscoelastic Layer viscoelastic layer of thickness e is interleaved (Fig. ). Material directions make an angle θ with the plate with the viscoelastic layers can be U = U +U + U + U 66,,,66 () The energies U and U are the strain energies directions, U is the coupling energy induced by the energy stored in the orthotropic layer and the strain energy stored in the viscoelastic layer. layers and 3 (Fig. ) can be written as () of the plate, and are the strain energies stored in layers and 3, are the reduced stiffness constants of the materials, and are functions of Fig. 37. Modeling of FRP Plate Using Ritz Method shown in Fig.. Among various passive damping layer of thickness e interleaved in the middle plane of laminates (Fig. ) and laminates with two viscoelastic layers of thickness e interleaved away from the middle plane (). The layers of the initial. Interlaminar Viscoelastic Layer viscoelastic layer of thickness e is interleaved (Fig. ). Material directions make an angle θ with the plate with the viscoelastic layers can be U = U +U + U + U 66,,,66 () The energies U and U are the strain energies directions, U is the coupling energy induced by the energy stored in the orthotropic layer and the strain energy stored in the viscoelastic layer. layers and 3 (Fig. ) can be written as () of the plate, and are the strain energies stored in layers and 3, are the reduced stiffness constants of the materials, and are functions of Fig. 37. Modeling of FRP Plate Using Ritz Method shown in Fig.. Among various passive damping layer of thickness e interleaved in the middle plane of laminates (Fig. ) and laminates with two viscoelastic layers of thickness e interleaved away from the middle plane (). The layers of the initial. Interlaminar Viscoelastic Layer viscoelastic layer of thickness e is interleaved (Fig. ). Material directions make an angle θ with the plate with the viscoelastic layers can be U = U +U + U + U 66,,,66 () The energies U and U are the strain energies directions, U is the coupling energy induced by the energy stored in the orthotropic layer and the strain energy stored in the viscoelastic layer. layers and 3 (Fig. ) can be written as () of the plate, and are the strain energies stored in layers and 3, are the reduced stiffness constants of the materials, and are functions of Fig. 37. Modeling of FRP Plate Using Ritz Method shown in Fig.. Among various passive damping layer of thickness e interleaved in the middle plane of laminates (Fig. ) and laminates with two viscoelastic layers of thickness e interleaved away from the middle plane (). The layers of the initial. Interlaminar Viscoelastic Layer viscoelastic layer of thickness e is interleaved (Fig. ). Material directions make an angle θ with the plate with the viscoelastic layers can be U = U +U + U + U 66,,,66 () The energies U and U are the strain energies directions, U is the coupling energy induced by the energy stored in the orthotropic layer and the strain energy stored in the viscoelastic layer. layers and 3 (Fig. ) can be written as () of the plate, and are the strain energies stored in layers and 3, are the reduced stiffness constants of the materials, and are functions of Fig. 37. Modeling of FRP Plate Using Ritz Method shown in Fig.. Among various passive damping layer of thickness e interleaved in the middle plane of laminates (Fig. ) and laminates with two viscoelastic layers of thickness e interleaved away from the middle plane (). The layers of the initial. Interlaminar Viscoelastic Layer viscoelastic layer of thickness e is interleaved (Fig. ). Material directions make an angle θ with the plate with the viscoelastic layers can be U = U +U + U + U 66,,,66 () The energies U and U are the strain energies directions, U is the coupling energy induced by the energy stored in the orthotropic layer and the strain energy stored in the viscoelastic layer. layers and 3 (Fig. ) can be written as () of the plate, and are the strain energies stored in layers and 3, are the reduced stiffness constants of the materials, and are functions of Fig. 37. Modeling of FRP Plate Using Ritz Method shown in Fig.. Among various passive damping layer of thickness e interleaved in the middle plane of laminates (Fig. ) and laminates with two viscoelastic layers of thickness e interleaved away from the middle plane (). The layers of the initial. Interlaminar Viscoelastic Layer viscoelastic layer of thickness e is interleaved (Fig. ). Material directions make an angle θ with the plate with the viscoelastic layers can be U = U +U + U + U 66,,,66 () The energies U and U are the strain energies directions, U is the coupling energy induced by the energy stored in the orthotropic layer and the strain energy stored in the viscoelastic layer. layers and 3 (Fig. ) can be written as () of the plate, and are the strain energies stored in layers and 3, are the reduced stiffness constants of the materials, and are functions of Fig. 37. Modeling of FRP Plate Using Ritz Method shown in Fig.. Among various passive damping layer of thickness e interleaved in the middle plane of laminates (Fig. ) and laminates with two viscoelastic layers of thickness e interleaved away from the middle plane (). The layers of the initial. Interlaminar Viscoelastic Layer viscoelastic layer of thickness e is interleaved (Fig. ). Material directions make an angle θ with the plate with the viscoelastic layers can be U = U +U + U + U 66,,,66 () The energies U and U are the strain energies directions, U is the coupling energy induced by the energy stored in the orthotropic layer and the strain energy stored in the viscoelastic layer. layers and 3 (Fig. ) can be written as () of the plate, and are the strain energies stored in layers and 3, are the reduced stiffness constants of the materials, and are functions of Fig.
4 Fig. where, the reduced stiffness constants are Poisson s ratio of the viscoelastic layer. This layer can be deduced by considering an orientation ; ; ; 4 ; ; (7). Two Interlaminar Viscoelastic Layers which two viscoelastic layers of thicknesses e are to be interleaved at distances d and d from the, layers can be Eqn. where is the strain energy stored in the orthotropic layers and layers, 3 and 5 can be Fig. where, the reduced stiffness constants are Poisson s ratio of the viscoelastic layer. This layer can be deduced by considering an orientation ; ; ; 4 ; ; (7). Two Interlaminar Viscoelastic Layers which two viscoelastic layers of thicknesses e are to be interleaved at distances d and d from the, layers can be Eqn. where is the strain energy stored in the orthotropic layers and layers, 3 and 5 can be Fig. where, the reduced stiffness constants are Poisson s ratio of the viscoelastic layer. This layer can be deduced by considering an orientation ; ; ; 4 ; ; (7). Two Interlaminar Viscoelastic Layers which two viscoelastic layers of thicknesses e are to be interleaved at distances d and d from the, layers can be Eqn. where is the strain energy stored in the orthotropic layers and layers, 3 and 5 can be Fig. where, the reduced stiffness constants are Poisson s ratio of the viscoelastic layer. This layer can be deduced by considering an orientation ; ; ; 4 ; ; (7). Two Interlaminar Viscoelastic Layers which two viscoelastic layers of thicknesses e are to be interleaved at distances d and d from the, layers can be Eqn. where is the strain energy stored in the orthotropic layers and layers, 3 and 5 can be Fig. where, the reduced stiffness constants are Poisson s ratio of the viscoelastic layer. This layer can be deduced by considering an orientation ; ; ; 4 ; ; (7). Two Interlaminar Viscoelastic Layers which two viscoelastic layers of thicknesses e are to be interleaved at distances d and d from the, layers can be Eqn. where is the strain energy stored in the orthotropic layers and layers, 3 and 5 can be Fig. where, the reduced stiffness constants are Poisson s ratio of the viscoelastic layer. This layer can be deduced by considering an orientation ; ; ; 4 ; ; (7). Two Interlaminar Viscoelastic Layers which two viscoelastic layers of thicknesses e are to be interleaved at distances d and d from the, layers can be Eqn. where is the strain energy stored in the orthotropic layers and layers, 3 and 5 can be Fig. where, the reduced stiffness constants are Poisson s ratio of the viscoelastic layer. This layer can be deduced by considering an orientation ; ; ; 4 ; ; (7). Two Interlaminar Viscoelastic Layers which two viscoelastic layers of thicknesses e are to be interleaved at distances d and d from the, layers can be Eqn. where is the strain energy stored in the orthotropic layers and layers, 3 and 5 can be Fig. where, the reduced stiffness constants are Poisson s ratio of the viscoelastic layer. This layer can be deduced by considering an orientation ; ; ; 4 ; ; (7). Two Interlaminar Viscoelastic Layers which two viscoelastic layers of thicknesses e are to be interleaved at distances d and d from the, layers can be Eqn. where is the strain energy stored in the orthotropic layers and layers, 3 and 5 can be Fig. where, the reduced stiffness constants are Poisson s ratio of the viscoelastic layer. This layer can be deduced by considering an orientation ; ; ; 4 ; ; (7). Two Interlaminar Viscoelastic Layers which two viscoelastic layers of thicknesses e are to be interleaved at distances d and d from the, layers can be Eqn. where is the strain energy stored in the orthotropic layers and layers, 3 and 5 can be Fig. where, the reduced stiffness constants are Poisson s ratio of the viscoelastic layer. This layer can be deduced by considering an orientation ; ; ; 4 ; ; (7). Two Interlaminar Viscoelastic Layers which two viscoelastic layers of thicknesses e are to be interleaved at distances d and d from the, layers can be Eqn. where is the strain energy stored in the orthotropic layers and layers, 3 and 5 can be Fig. where, the reduced stiffness constants are Poisson s ratio of the viscoelastic layer. This layer can be deduced by considering an orientation ; ; ; 4 ; ; (7). Two Interlaminar Viscoelastic Layers which two viscoelastic layers of thicknesses e are to be interleaved at distances d and d from the, layers can be Eqn. where is the strain energy stored in the orthotropic layers and layers, 3 and 5 can be
5 39 () pq =,,,66 () layers and 4 can be written as () where, the functions are given by Eq.. In In the case of a beam clamped at the end x = and At the end x = : x, x,, (7),, (8) free beam are listed in Table with the corresponding.5π,,,, (), 3 () translation and rotation. The two roots λ = and λ = are associated with these functions. The other roots values of λ m and γ m are given in Table for m varying from to 9. The first mode of free vibrations is 39 () pq =,,,66 () layers and 4 can be written as () where, the functions are given by Eq.. In In the case of a beam clamped at the end x = and At the end x = : x, x,, (7),, (8) free beam are listed in Table with the corresponding.5π,,,, (), 3 () translation and rotation. The two roots λ = and λ = are associated with these functions. The other roots values of λ m and γ m are given in Table for m varying from to 9. The first mode of free vibrations is 39 () pq =,,,66 () layers and 4 can be written as () where, the functions are given by Eq.. In In the case of a beam clamped at the end x = and At the end x = : x, x,, (7),, (8) free beam are listed in Table with the corresponding.5π,,,, (), 3 () translation and rotation. The two roots λ = and λ = are associated with these functions. The other roots values of λ m and γ m are given in Table for m varying from to 9. The first mode of free vibrations is 39 () pq =,,,66 () layers and 4 can be written as () where, the functions are given by Eq.. In In the case of a beam clamped at the end x = and At the end x = : x, x,, (7),, (8) free beam are listed in Table with the corresponding.5π,,,, (), 3 () translation and rotation. The two roots λ = and λ = are associated with these functions. The other roots values of λ m and γ m are given in Table for m varying from to 9. The first mode of free vibrations is 39 () pq =,,,66 () layers and 4 can be written as () where, the functions are given by Eq.. In In the case of a beam clamped at the end x = and At the end x = : x, x,, (7),, (8) free beam are listed in Table with the corresponding.5π,,,, (), 3 () translation and rotation. The two roots λ = and λ = are associated with these functions. The other roots values of λ m and γ m are given in Table for m varying from to 9. The first mode of free vibrations is 39 () pq =,,,66 () layers and 4 can be written as () where, the functions are given by Eq.. In In the case of a beam clamped at the end x = and At the end x = : x, x,, (7),, (8) free beam are listed in Table with the corresponding.5π,,,, (), 3 () translation and rotation. The two roots λ = and λ = are associated with these functions. The other roots values of λ m and γ m are given in Table for m varying from to 9. The first mode of free vibrations is 39 () pq =,,,66 () layers and 4 can be written as () where, the functions are given by Eq.. In In the case of a beam clamped at the end x = and At the end x = : x, x,, (7),, (8) free beam are listed in Table with the corresponding.5π,,,, (), 3 () translation and rotation. The two roots λ = and λ = are associated with these functions. The other roots values of λ m and γ m are given in Table for m varying from to 9. The first mode of free vibrations is 39 () pq =,,,66 () layers and 4 can be written as () where, the functions are given by Eq.. In In the case of a beam clamped at the end x = and At the end x = : x, x,, (7),, (8) free beam are listed in Table with the corresponding.5π,,,, (), 3 () translation and rotation. The two roots λ = and λ = are associated with these functions. The other roots values of λ m and γ m are given in Table for m varying from to 9. The first mode of free vibrations is 39 () pq =,,,66 () layers and 4 can be written as () where, the functions are given by Eq.. In In the case of a beam clamped at the end x = and At the end x = : x, x,, (7),, (8) free beam are listed in Table with the corresponding.5π,,,, (), 3 () translation and rotation. The two roots λ = and λ = are associated with these functions. The other roots values of λ m and γ m are given in Table for m varying from to 9. The first mode of free vibrations is 39 () pq =,,,66 () layers and 4 can be written as () where, the functions are given by Eq.. In In the case of a beam clamped at the end x = and At the end x = : x, x,, (7),, (8) free beam are listed in Table with the corresponding.5π,,,, (), 3 () translation and rotation. The two roots λ = and λ = are associated with these functions. The other roots values of λ m and γ m are given in Table for m varying from to 9. The first mode of free vibrations is 39 () pq =,,,66 () layers and 4 can be written as () where, the functions are given by Eq.. In In the case of a beam clamped at the end x = and At the end x = : x, x,, (7),, (8) free beam are listed in Table with the corresponding.5π,,,, (), 3 () translation and rotation. The two roots λ = and λ = are associated with these functions. The other roots values of λ m and γ m are given in Table for m varying from to 9. The first mode of free vibrations is
6 4 Table Coefficients of a clampedfree beam function. m λ m γ m ((m.5)π Plate with two free ends Fig. 5 Free Free Beam condition. Length (a) = 3 mm Breadth (b) = mm No of plies (n) = 8 Thickness of each ply (t) =.3 mm Force (q ) = 5 N Thickness of Viscoelastic material (e ) =. mm The materials properties of chosen materials listed in Table Results and Discussion Loss factor (η) of unidirectional carbon fibre/epoxy laminate with different boundary conditions and at various fibre orientations for a single and multiple viscoelastic layer positions from the laminate mid plane. Case I: (CFFF) One edge clamped all other edges free. Case II: (CCCC) All edges clamped. Case III: (CFCF) Adjacent edges clamped. The loss factor (η) of Unidirectional Carbon Fibres/Epoxy with different boundary conditions and at various fibre orientations without and with Viscoelastic Layers is shown in Table 4. and Table 5 respevtively. Figs 6 and 7 are the plot of results displayed in Tables 4 and 5 i.e loss factor as a function of fiber orientation. Table Coefficients of a freefree beam function. m λ m γ m Table 3 Materials properties of glass/epoxy and viscoelastic layer. E L E T Material (GPa) (GPa) G LT (GPa) υ LT % % % Carbon/Epoxy Viscoelastic 5 (MPa) 5 (MPa) 5 (Mpa) Table 4 Loss factor (η) of unidirectional carbon fibres/epoxy with different boundary conditions and at various fibre orientations without viscoelastic layers. Angle CCCC CFFF CFCF
7 4 Table 5 Loss factor (η) of unidirectional carbon fibres/epoxy with CFCF boundary conditions and at various fibre orientations with viscoelastic layers. Angle Loss factor (η) of carbon/ epoxy laminate CFCF Mid Sym Asym Outer Loss Factor Fibre Orientation Fig. 6 Variation of Loss factor (η) of unidirectional carbon fibres with fibre orientation without viscoelastic layers. Loss Factor CCCC CFFF CFCF Midplane.6 Symm Asymm Outer Fibre Orientation Fig. 7 Loss factor (η) of unidirectional carbon fibres (CFCF) with viscoelastic material inserted at various positions with fibre orientation. 6. Conclusions This study investigates the damping properties of unidirectional carbon reinforced laminates shows very poor damping values when compared with glass and Kevlar reinforced laminates [3]. But, when it is provided with interleaved constrain layer with a single or two its damping values obtain are considerably high. For a given laminate without constrain layer, the CFCF (Fig. 6) will have maximum value of loss factor at 6. Whereas the minimum value for the same boundary conditions recorded at 5 if a constrain layer is used at midplane position. For all other positions of constrain layer the loss factor is in between.5% at 3 single midplane to.97% at 9 two outer position. It shows that damping nature of carbon laminates and 9 enhanced four folds. It is also realized that the provision of constrain layer in the FRP lamination process is highly compatible. It is noticed that a trend of increase in the damping of laminates significant as the viscoelastic layers are placed from the mid layer to outer layer. Also it showed that, the least value of loss factor found at 3 when two layers are used irrespective of their locations. References [] Adams, R. D. and Maheri, M. R Dynamic Flexural Properties of Anisotropic FIbrous Composite Beams. Compos Sci Technol 5 : [] Billups, E. K. and Cavalli, M. N. 7. DDamping Predictions of Fibre Composite Plates: Layup Effects. Compos. Sci. Technol. 68 :
8 4 [3] Maheri, A. M., Assarar, M., Sefrani, Y. and Berthelot, J.M. 8. Damping Analysis of Orthotropic Composite Materials and Laminates Composites. 39: [4] Berthelot, J.M. and Sefrani, Y. 4. Damping Analysis of Unidirectional Glass and Kevlar Fibre Composites. Composites Science and Technology 64: [5] Li, J.Q. and Narita, Y. 3. Analysis and Optimal Design for the Damping Property of Laminated Viscoelastic Plates under General Edge Conditions. Composites: Part B 45: [6] Berthelot, J.M. 6. Damping Analysis of Orthotropic Composites with Interleaved Viscoelastic Layers: Modelling. Journal of Composite Materials 4 (): [7] Ni, R. G. and Adams, R. D The Damping and Dynamic Moduli of Symmetric Laminated Composite BeamsTheoretical and Experimental Results. J. Compos Mater 8 (): 4.
Passive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationVIBRATION CONTROL OF RECTANGULAR CROSSPLY FRP PLATES USING PZT MATERIALS
Journal of Engineering Science and Technology Vol. 12, No. 12 (217) 33983411 School of Engineering, Taylor s University VIBRATION CONTROL OF RECTANGULAR CROSSPLY FRP PLATES USING PZT MATERIALS DILEEP
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationEffect of magnetostrictive material layer on the stress and deformation behaviour of laminated structure
IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS Effect of magnetostrictive material layer on the stress and deformation behaviour of laminated structure To cite this article:
More informationDynamic analysis of Composite Micro Air Vehicles
Dynamic analysis of Composite Micro Air Vehicles Shishir Kr. Sahu Professor and Head, Civil Engineering, National Institute of Technology, Rourkela, India Email: sksahu@nitrkl.ac.in ABSTRACT The present
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationDynamic Analysis of Laminated Composite Plate Structure with Square CutOut under Hygrothermal Load
Dynamic Analysis of Laminated Composite Plate Structure with Square CutOut under Hygrothermal Load Arun Mukherjee 1, Dr. Sreyashi Das (nee Pal) 2 and Dr. A. Guha Niyogi 3 1 PG student, 2 Asst. Professor,
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationI INTRODUCTION II THEORY
Estimation of Loss Factor of Viscoelastic Material by Using Cantilever Sandwich Plate 1 Jitender Kumar, 2 Dr. Rajesh Kumar 1 Geeta Engineering College (Panipat) 2 SLIET Longowal, Punjab 1 jitd2007@rediffmail.com
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationFrequency Response of Composite Laminates at Various Boundary Conditions
International Journal of Engineering Science Invention (IJESI) ISSN (Online): 2319 6734, ISSN (Print): 2319 6726 www.ijesi.org ǁ PP.1115 Frequency Response of Composite Laminates at Various Boundary Conditions
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationModule 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations
Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates CrossPly Laminates Specially Orthotropic Laminates Examples Homework References
More informationAmerican Society for Testing and Materials (ASTM) Standards. Mechanical Testing of Composites and their Constituents
Mechanical Testing of Composites and their Constituents American Society for Testing and Materials (ASTM) Standards Tests done to determine intrinsic material properties such as modulus and strength for
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationPrediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach
Prediction of the Ultimate Strength of Composite Laminates Under InPlane Loading Prediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach Tae Jin
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationNUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET
NUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET M.Gümüş a*, B.Gözlüklü a, D.Çöker a a Department of Aerospace Eng., METU, Ankara, Turkey *mert.gumus@metu.edu.tr Keywords:
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More informationPLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
More informationPrediction of Micromechanical Behaviour of Elliptical Frp Composites
Prediction of Micromechanical Behaviour of Elliptical Frp Composites Kiranmayee.Nerusu Dept. of Mechanical Engg. P. V. P. Siddhartha Institute of Technology, Vijayawada 520 007, A.P, India. P. Phani Prasanthi
More informationComposite Materials Research Laboratory, State University of New York at Buffalo, Buffalo, NY , USA
Composite Interfaces, Vol. 7, No. 4, pp. 257 275 (2000) VSP 2000. Discontinuous surfacetreated submicrondiameter carbon filaments as an interlaminar filler in carbon fiber polymermatrix composites for
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationSTUDY OF THE EFFECT OF COMPOSITE CONSTRAINED LAYERS IN VIBRATION DAMPING OF PLATES
Int. J. of Applied Mechanics and Engineering, 214, vol.19, No.1, pp.2329 DOI: 1.2478/ijame21415 Brief note STUDY OF THE EFFECT OF COMPOSITE CONSTRAINED LAYERS IN VIBRATION DAMPING OF PLATES K.S.K. SASIKUMAR
More informationDynamic Response Of Laminated Composite Shells Subjected To Impulsive Loads
IOSR Journal of Mechanical and Civil Engineering (IOSRJMCE) eissn: 22781684,pISSN: 2320334X, Volume 14, Issue 3 Ver. I (May.  June. 2017), PP 108123 www.iosrjournals.org Dynamic Response Of Laminated
More informationA copy can be downloaded for personal noncommercial research or study, without prior permission or charge
York, C. B. (2015) Influence of bending twisting coupling on compression and shear buckling strength. Stability of Structures 14th Symposium, Zakopane, Poland, 812 Jun 2015. Copyright 2015 The Author.
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationFailure Analysis of Unidirectional Composite Pinned Joints
217 IJEDR Volume, Issue 4 ISSN: 23219939 Failure Analysis of Unidirectional Composite Pinned Joints 1 Sai Ashok.M, 2 Mr. U. Koteswara Rao 1 Mtech Machine Design, 2 Associate Professor & Asst. COE 1
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationVibration Modelling of Composite Laminates with Delamination Damage
Proceedings of 20 th International Congress on Acoustics, ICA 2010 2327 August 2010, Sydney, Australia Vibration Modelling of Composite Laminates with Delamination Damage Z. Zhang, K. Shankar, M. Tahtali
More informationDesign of Hybrid Composites for Axial loads with Zero Coefficient of Thermal Expansion
Design of Hybrid Composites for Axial loads with Zero Coefficient of Thermal Expansion Zaffar M. Khan 1 and Asim Shahzad 2 Institute of Space Technology, Islamabad, Pakistan, 44000 Aerospace structures
More informationAnalysis of Flexural Properties of Carbon Fiber Reinforced / EPoxy Composite Material
ISSN 23951621 Analysis of Flexural Properties of Carbon Fiber Reinforced / EPoxy Composite Material #1 Kishor Shingare, #2 Dr. S.M. Shendokar, #3 Prof. P.V. Deshmukh, #4 Prof. S.S. Chavan 1 kishorshingare911@gmail.com
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationINTERNAL STRAIN MEASUREMENTS IN CFRP PLATES SUBJECTED TO IMPACT LOAD USING FBG SENSORS
INTERNAL STRAIN MEASUREMENTS IN CFRP PLATES SUBJECTED TO IMPACT LOAD USING FBG SENSORS J. Frieden, J. Cugnoni, J. Botsis, Th. Gmür, D. Coric Laboratoire de Mécanique appliquée et d Analyse de Fiabilité
More informationVIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS
VIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS Mechanical Engineering Department, Indian Institute of Technology, New Delhi 110 016, India (Received 22 January 1992,
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationTheoretical Approach to Predict Transverse Impact Response of VariableStiffness Curved Composite Plates
*Manuscript Click here to view linked References 1 1 1 1 1 1 1 0 1 0 1 0 1 0 1 0 1 Theoretical Approach to Predict Transverse Impact Response of VariableStiffness Curved Composite Plates B. Arachchige,
More informationA Numerical Study on Prediction of BFS in Composite Structures under Ballistic Impact
VOL. 1, 2015 ISSN 2394 3750 EISSN 2394 3769 SCIENCE & TECHNOLOGY A Numerical Study on Prediction of BFS in Composite Structures under Ballistic Impact Bandaru Aswani Kumar 1, Suhail Ahmad 2 1. Research
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationDEVELOPMENT OF THERMOELASTIC STRESS ANALYSIS AS A NONDESTRUCTIVE EVALUATION TOOL
DEVELOPMENT OF THERMOELASTIC STRESS ANALYSIS AS A NONDESTRUCTIVE EVALUATION TOOL S. Quinn*, R.K. Fruehmann and J.M. DulieuBarton School of Engineering Sciences University of Southampton Southampton SO17
More informationInfluence of Inherent Material Damping on the Dynamic Buckling of Composite Columns with Open Cross Sections
Mechanics and Mechanical Engineering Vol. 17, No. 1 (2013) 59 69 c Lodz University of Technology Influence of Inherent Material Damping on the Dynamic Buckling of Composite Columns with Open Cross Sections
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationNumerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive Zone Model
Numerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive Zone Model Numerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive
More informationON THE NUMERICAL ANALYSIS OF COMPOSITE MATERIAL
The 4th International Conference Advanced Composite Materials Engineering COMAT 8 October, Brasov, Romania O THE UMERICAL AALYSIS OF COMPOSITE MATERIAL D.D. icoara Transilvania University, City Brasov,
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationFree Vibration Response of a Multilayer Smart Hybrid Composite Plate with Embedded SMA Wires
11(2014) 279298 Free Vibration Response of a Multilayer Smart Hybrid Composite Plate with Embedded SMA Wires Abstract In this paper, free vibration response of a hybrid composite plate was studied. Effects
More informationOPTIMAL FIBER PLACEMENT INCLUDING EFFECTS OF EMBROIDERY
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS OPTIMAL FIBER PLACEMENT INCLUDING EFFECTS OF EMBROIDERY T. Nishida 1 T. Ieda 2 * A. Senba 2 1 Department of Aerospace Engineering Nagoya University
More informationInfluence of fibre proportion and position on the machinability of GFRP composites An FEA model
Indian Journal of Engineering & Materials Sciences Vol. 12, October 2005, pp. 443450 Influence of fibre proportion and position on the machinability of GFRP composites An FEA model D Abdul Budan* Department
More informationDYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.1419:628.183=20 DYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES J. ESKANDARI JAM 1 and N. GARSHASBI NIA 2 1 Aerospace
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationAnalysis Of Naca 2412 For Automobile Rear Spoiler Using Composite Material *
Analysis Of Naca 2412 For Automobile Rear Spoiler Using Composite Material * Kamprasad Chodagudi 1, T.b.s Rao 2 
More informationCOMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD
10th International DAAAM Baltic Conference "INDUSTRIAL ENGINEERING  1213 May 2015, Tallinn, Estonia COMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD Sedláček,
More informationEFFECTIVENESS OF NANO LAYERS ON INTERLAMINAR STREESES OF COMPOSITE LAMINATE
International Journal of Mechanical Engineering and Technology (IJMET) Volume, Issue 1, January 217, pp. 15 2, Article ID: IJMET 1_2 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=&itype=1
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationEVALUATION OF THERMAL CYCLING INFLUENCE ON PEI/CARBON FIBER COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF THERMAL CYCLING INFLUENCE ON PEI/CARBON FIBER COMPOSITES N.L. Batista 1, K. Iha 1, E.C. Botelho * 1 Department of Chemistry, Technological
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationSSRG International Journal of Mechanical Engineering (SSRGIJME) volume1 issue5 September 2014
Finite Element Modeling for Delamination Analysis of Double Cantilever Beam Specimen Mohammed Waseem H.S. 1, Kiran Kumar N. 2 1 Post Graduate Student, 2 Asst. Professor Dept. of Mechanical Engineering,
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationDesign of Automobile Driveshaft using Carbon/Epoxy and Kevlar/Epoxy Composites
American Journal of Engineering Research (AJER) eissn : 23200847 pissn : 23200936 Volume02, Issue10, pp173179 www.ajer.org Research Paper Open Access Design of Automobile Driveshaft using Carbon/Epoxy
More informationFinite element analysis of drilled holes in unidirectional composite laminates using failure theories
American Journal of Science and Technology 2014; 1(3): 101105 Published online May 30, 2014 (http://www.aascit.org/journal/ajst) Finite element analysis of drilled holes in unidirectional composite laminates
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationFLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR DEFORMABLE PLATE THEORY
AsiaPacific Conference on FRP in Structures (APFIS 2007) S.T. Smith (ed) 2007 International Institute for FRP in Construction FLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationFinite Element and Plate Theory Modeling of Acoustic Emission Waveforms. NASA Langley Research Center. Hampton, VA *University of Denver
Finite Element and Plate Theory Modeling of Acoustic Emission Waveforms W. H. Prosser, M. A. Hamstad + *, J. Gary +, and A. O Gallagher + NASA Langley Research Center Hampton, VA 236811 *University of
More informationANALYTICAL SOLUTIONS USING HIGH ORDER COMPOSITE LAMINATE THEORY FOR HONEYCOMB SANDWICH PLATES WITH VISCOELASTIC FREQUENCY DEPENDENT DAMPING
Clemson University TigerPrints All Theses Theses 811 ANALYTICAL SOLUTIONS USING HIGH ORDER COMPOSITE LAMINATE THEORY FOR HONEYCOMB SANDWICH PLATES WITH VISCOELASTIC FREQUENCY DEPENDENT DAMPING Nan Shan
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationMaterial Characterization of Carbon Fiber Reinforced Polymer Laminate Using Virtual Fields Method
Proceedings of ICTACEM 014 International Conference on Theoretical, Applied, Computational and Experimental Mechanics December 931, 014, IIT Kharagpur, India ICTACEM014/39 Material Characterization of
More informationEXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS
EXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS Umar Farooq and Karl Gregory School of Built Environment and Department of Engineering, University of Bolton,
More informationIJSER 1. INTRODUCTION. M.Elhadary
1591 A new failure criterion for GRP composite materials subjected to inphase and outofphase biaxial fatigue loading under different stress ratios M.Elhadary Abstract this studying the fatigue behavior
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationThermal buckling and postbuckling of laminated composite plates with. temperature dependent properties by an asymptotic numerical method
hermal buckling and postbuckling of laminated composite plates with temperature dependent properties by an asymptotic numerical method F. Abdoun a,*, L. Azrar a,b, E.M. Daya c a LAMA, Higher School of
More informationNumerical Vibration Analysis of Impacted CFRP Specimens Using COMSOL Multiphysics
Numerical Vibration Analysis of Impacted CFRP Specimens Using COMSOL Multiphysics Philipp Jatzlau 1, Florian Seybold 1 1 Technical University of Munich, Center for Building Materials, Chair of Nondestructive
More informationIDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE
IDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE Hugo Sol, hugos@vub.ac.be Massimo Bottiglieri, Massimo.Bottiglieri@vub.ac.be Department Mechanics of Materials
More information